#------------------------------------------------------------------------------
#$Date: 2016-03-22 11:41:31 +0100 (mar 22 de mar de 2016) $
#$Revision: 178959 $
#$URL: svn://www.crystallography.net/cod/cif/4/11/88/4118882.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4118882
loop_
_publ_author_name
'Hong-Ling Cai'
'Yi Zhang'
'Da-Wei Fu'
'Wen Zhang'
'Tao Liu'
'Hirofumi Yoshikawa'
'Kunio Awaga'
'Ren-Gen Xiong'
_publ_section_title
;
 Above-Room-Temperature Magnetodielectric Coupling in a Possible
 Molecule-Based Multiferroic: Triethylmethylammonium
 Tetrabromoferrate(III)
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              18487
_journal_page_last               18490
_journal_paper_doi               10.1021/ja3073319
_journal_volume                  134
_journal_year                    2012
_chemical_formula_sum            'C7 H18 Br4 Fe N'
_chemical_formula_weight         491.71
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   8.344(9)
_cell_length_b                   8.344(9)
_cell_length_c                   13.67(2)
_cell_measurement_reflns_used    542
_cell_measurement_temperature    363(2)
_cell_measurement_theta_max      27.5
_cell_measurement_theta_min      2.5
_cell_volume                     824.2(17)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      363(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.1046
_diffrn_reflns_av_sigmaI/netI    0.0521
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       9
_diffrn_reflns_limit_k_min       -9
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            6657
_diffrn_reflns_theta_full        24.49
_diffrn_reflns_theta_max         24.49
_diffrn_reflns_theta_min         2.82
_exptl_absorpt_coefficient_mu    10.582
_exptl_absorpt_correction_T_max  1.0
_exptl_absorpt_correction_T_min  0.9
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   crystalclear
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    1.982
_exptl_crystal_description       block
_exptl_crystal_F_000             466
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.1
_exptl_crystal_size_min          0.1
_refine_diff_density_max         1.100
_refine_diff_density_min         -0.502
_refine_diff_density_rms         0.180
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.16(3)
_refine_ls_extinction_coef       0.0331(18)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.139
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     26
_refine_ls_number_reflns         569
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.138
_refine_ls_R_factor_all          0.1064
_refine_ls_R_factor_gt           0.0813
_refine_ls_shift/su_max          0.042
_refine_ls_shift/su_mean         0.010
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1174P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1869
_refine_ls_wR_factor_ref         0.2063
_reflns_number_gt                418
_reflns_number_total             569
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja3073319_si_006.cif
_cod_data_source_block           1
_cod_original_cell_volume        824.1(18)
_cod_database_code               4118882
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'x-y, x, z+1/2'
'-y, x-y, z'
'-x, -y, z+1/2'
'-x+y, -x, z'
'y, -x+y, z+1/2'
'y, x, z+1/2'
'-x+y, y, z'
'-x, -x+y, z+1/2'
'-y, -x, z'
'x-y, -y, z+1/2'
'x, x-y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
N1 N -0.3333 -0.6667 0.7736(12) 0.118(2) Uani 1 6 d S
C1 C -0.113(2) -0.474(2) 0.7709(19) 0.118(2) Uani 0.33 1 d P
H1A H -0.0651 -0.4605 0.8368 0.141 Uiso 0.35 1 d PR
H1B H -0.1206 -0.3638 0.7560 0.141 Uiso 0.35 1 d PR
C2 C -0.005(3) -0.5025(14) 0.7274(9) 0.118(2) Uani 0.67 2 d SP
H2A H 0.1161 -0.3927 0.7323 0.176 Uiso 0.36 1 d PR
H2B H 0.0043 -0.6108 0.7429 0.176 Uiso 0.36 1 d PR
H2C H -0.0518 -0.5239 0.6614 0.176 Uiso 0.72 2 d SPR
C3 C -0.2791(10) -0.7209(10) 0.8377(10) 0.118(2) Uani 0.67 2 d SP
H3A H -0.1457 -0.6729 0.8357 0.141 Uiso 0.35 1 d PR
H3B H -0.3341 -0.8613 0.8357 0.141 Uiso 0.35 1 d PR
C4 C -0.3333 -0.6667 0.9557(12) 0.118(2) Uani 1 6 d S
H4A H -0.2924 -0.7076 1.0118 0.176 Uiso 0.34 2 d SPR
H4B H -0.2772 -0.5544 0.9573 0.176 Uiso 0.34 2 d SPR
H4C H -0.4669 -0.7334 0.9573 0.176 Uiso 0.34 2 d SPR
Fe1 Fe 0.0000 0.0000 1.02405(10) 0.0696(4) Uani 1 6 d S
Br1 Br 0.0000 0.0000 1.19342(10) 0.1162(5) Uani 1 6 d S
Br2 Br 0.15232(6) -0.15232(6) 0.96873(8) 0.1197(3) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Br Br -0.2901 2.4595 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Fe Fe 0.3463 0.8444 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
C3 N1 C3 70.5(14) . 3_445
C3 N1 C3 70.5(14) . 5_545
C3 N1 C3 70.5(14) 3_445 5_545
C3 N1 C1 58.7(10) . 5_545
C3 N1 C1 128.8(14) 3_445 5_545
C3 N1 C1 86.6(9) 5_545 5_545
C3 N1 C1 58.7(10) . 12_545
C3 N1 C1 86.6(9) 3_445 12_545
C3 N1 C1 128.8(14) 5_545 12_545
C1 N1 C1 72.9(14) 5_545 12_545
C3 N1 C1 86.6(9) . .
C3 N1 C1 58.7(10) 3_445 .
C3 N1 C1 128.8(15) 5_545 .
C1 N1 C1 119.95(8) 5_545 .
C1 N1 C1 47.1(15) 12_545 .
C3 N1 C1 86.6(9) . 10_445
C3 N1 C1 128.8(14) 3_445 10_445
C3 N1 C1 58.7(10) 5_545 10_445
C1 N1 C1 47.1(15) 5_545 10_445
C1 N1 C1 119.95(8) 12_545 10_445
C1 N1 C1 166.9(15) . 10_445
C3 N1 C1 128.8(14) . 8
C3 N1 C1 58.7(10) 3_445 8
C3 N1 C1 86.6(9) 5_545 8
C1 N1 C1 166.9(15) 5_545 8
C1 N1 C1 119.95(9) 12_545 8
C1 N1 C1 72.9(15) . 8
C1 N1 C1 119.95(8) 10_445 8
C3 N1 C1 128.8(14) . 3_445
C3 N1 C1 86.6(9) 3_445 3_445
C3 N1 C1 58.7(10) 5_545 3_445
C1 N1 C1 119.95(8) 5_545 3_445
C1 N1 C1 166.9(15) 12_545 3_445
C1 N1 C1 119.95(8) . 3_445
C1 N1 C1 72.9(15) 10_445 3_445
C1 N1 C1 47.1(15) 8 3_445
C2 C1 C1 54.8(10) . 12_545
C2 C1 C3 144.2(18) . 3_445
C1 C1 C3 89.4(9) 12_545 3_445
C2 C1 N1 112.1(16) . .
C1 C1 N1 66.4(7) 12_545 .
C3 C1 N1 41.8(8) 3_445 .
C2 C1 C3 102.5(14) . .
C1 C1 C3 47.7(8) 12_545 .
C3 C1 C3 41.7(10) 3_445 .
N1 C1 C3 35.2(6) . .
C2 C1 H1A 99.8 . .
C1 C1 H1A 84.5 12_545 .
C3 C1 H1A 73.9 3_445 .
N1 C1 H1A 105.8 . .
C3 C1 H1A 74.4 . .
C2 C1 H1B 119.6 . .
C1 C1 H1B 167.4 12_545 .
C3 C1 H1B 95.4 3_445 .
N1 C1 H1B 110.2 . .
C3 C1 H1B 136.0 . .
H1A C1 H1B 107.9 . .
C1 C2 C1 70(2) . 12_545
C1 C2 H2A 108.0 . .
C1 C2 H2A 142.9 12_545 .
C1 C2 H2B 119.9 . .
C1 C2 H2B 51.4 12_545 .
H2A C2 H2B 109.5 . .
C1 C2 H2C 103.0 . .
C1 C2 H2C 104.2 12_545 .
H2A C2 H2C 112.0 . .
H2B C2 H2C 104.3 . .
N1 C3 C3 54.7(7) . 5_545
N1 C3 C3 54.7(7) . 3_445
C3 C3 C3 60.000(4) 5_545 3_445
N1 C3 C1 79.6(11) . 5_545
C3 C3 C1 90.6(9) 5_545 5_545
C3 C3 C1 133.9(9) 3_445 5_545
N1 C3 C1 79.6(11) . 12_545
C3 C3 C1 133.9(9) 5_545 12_545
C3 C3 C1 90.6(9) 3_445 12_545
C1 C3 C1 86.3(19) 5_545 12_545
N1 C3 C4 112.3(12) . .
C3 C3 C4 67.8(4) 5_545 .
C3 C3 C4 67.8(4) 3_445 .
C1 C3 C4 136.3(10) 5_545 .
C1 C3 C4 136.3(10) 12_545 .
N1 C3 C1 58.2(7) . 10_445
C3 C3 C1 47.7(8) 5_545 10_445
C3 C3 C1 99.9(7) 3_445 10_445
C1 C3 C1 42.9(14) 5_545 10_445
C1 C3 C1 115.1(16) 12_545 10_445
C4 C3 C1 106.1(9) . 10_445
N1 C3 C1 58.2(7) . .
C3 C3 C1 100.0(7) 5_545 .
C3 C3 C1 47.7(8) 3_445 .
C1 C3 C1 115.1(16) 5_545 .
C1 C3 C1 42.9(14) 12_545 .
C4 C3 C1 106.1(9) . .
C1 C3 C1 115.5(14) 10_445 .
N1 C3 H3A 113.5 . .
C3 C3 H3A 159.1 5_545 .
C3 C3 H3A 99.2 3_445 .
C1 C3 H3A 104.8 5_545 .
C1 C3 H3A 36.5 12_545 .
C4 C3 H3A 107.6 . .
C1 C3 H3A 145.6 10_445 .
C1 C3 H3A 60.9 . .
N1 C3 H3B 112.4 . .
C3 C3 H3B 97.1 5_545 .
C3 C3 H3B 157.1 3_445 .
C1 C3 H3B 36.2 5_545 .
C1 C3 H3B 106.4 12_545 .
C4 C3 H3B 106.8 . .
C1 C3 H3B 59.2 10_445 .
C1 C3 H3B 146.7 . .
H3A C3 H3B 103.6 . .
C3 C4 C3 44.5(9) . 5_545
C3 C4 C3 44.5(9) . 3_445
C3 C4 C3 44.5(9) 5_545 3_445
C3 C4 H4A 116.5 . .
C3 C4 H4A 147.8 5_545 .
C3 C4 H4A 147.8 3_445 .
C3 C4 H4B 104.1 . .
C3 C4 H4B 104.1 5_545 .
C3 C4 H4B 65.7 3_445 .
H4A C4 H4B 106.4 . .
C3 C4 H4C 103.9 . .
C3 C4 H4C 65.4 5_545 .
C3 C4 H4C 103.9 3_445 .
H4A C4 H4C 106.6 . .
H4B C4 H4C 119.9 . .
Br1 Fe1 Br2 108.96(5) . 5
Br1 Fe1 Br2 108.96(5) . 3
Br2 Fe1 Br2 109.98(5) 5 3
Br1 Fe1 Br2 108.96(5) . .
Br2 Fe1 Br2 109.98(5) 5 .
Br2 Fe1 Br2 109.98(5) 3 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
N1 C3 1.175(18) .
N1 C3 1.175(18) 3_445
N1 C3 1.175(18) 5_545
N1 C1 1.735(13) 5_545
N1 C1 1.735(13) 12_545
N1 C1 1.735(14) .
N1 C1 1.735(14) 10_445
N1 C1 1.735(13) 8
N1 C1 1.735(13) 3_445
C1 C2 1.20(3) .
C1 C1 1.39(4) 12_545
C1 C3 1.51(2) 3_445
C1 C3 2.04(2) .
C1 H1A 0.9693 .
C1 H1B 0.9691 .
C2 C1 1.20(3) 12_545
C2 H2A 0.9695 .
C2 H2B 0.9685 .
C2 H2C 0.9636 .
C3 C3 1.36(3) 5_545
C3 C3 1.36(3) 3_445
C3 C1 1.51(2) 5_545
C3 C1 1.51(2) 12_545
C3 C4 1.79(2) .
C3 C1 2.04(2) 10_445
C3 H3A 0.9768 .
C3 H3B 1.0228 .
C4 C3 1.79(2) 5_545
C4 C3 1.79(2) 3_445
C4 H4A 0.9693 .
C4 H4B 0.8118 .
C4 H4C 0.9651 .
Fe1 Br1 2.315(4) .
Fe1 Br2 2.328(3) 5
Fe1 Br2 2.328(3) 3
Fe1 Br2 2.328(3) .
